Presentation on theme: "GOVERNMENT COLLEGE OF ENGINEERING, SALEM."— Presentation transcript:
1GOVERNMENT COLLEGE OF ENGINEERING, SALEM. CAST IRONPRESENTED BYJEEVA.TYASODHA.M
2INTRODUCTIONCast iron usually refers to grey iron, but also identifies a large group of ferrous alloys, which solidify with a eutectic.Cast iron tends to be brittle, except for malleable cast irons.The color of a fractured surface can be used to identify an alloy.
3CONTENTS CAST IRON. CLASSIFICATION. APPLICATIONS OF CAST IRONS. WHITE.MALLEABLE.GRAY.DUCTILE.APPLICATIONS OF CAST IRONS.HEAT TREATING TO CONTROL STRUCTURE.
4ABOUT CAST IRON Family of ferrous alloys. Cast into desired shape – not worked.2-4% C and 1-3% Si.Instability of Fe3C:Cementite / graphite flakes / graphite nodules.
5TYPES OF CAST IRON Alloying elements. Grey cast iron. White cast iron. Malleable cast iron.Ductile cast iron.
9CLASSIFICATION OF CAST IRON S.NOTYPES OF CAST IRONGRAPHITEDUCTILITYPROPERTY1WHITENOFAST COOLING RATES2GRAYFlakeSLOW COOLING RATES3MALLEABLEAnneal:flake tonoduleYESWHITE IRON + ANNEALINGHEAT TREATMENT4NODULARNodularADDITIONS MADE SO THATNODULES OF GRAPHITEFORM INSTEAD OF FLAKES
10FACTORS INFLUENCING WHICH WILL FORM TEMPERATURE (COOLING RATE)
13GREY VS NODULAR CAST IRON (X250) FerriticpearliticGray – graphite as Nodular – graphite as Flakes nodulesBrittle Ductile
14WHITE CAST IRON Fe3 C+ pearlite. Hard, brittle. Shows a “white” crystalline fractured surface. Excellent wear resistance. High compressive stress.
15MALLEABLE CAST IRON White cast iron + annealing treatment. During annealing treatment graphite nucleates and grows from the Fe3C to form nodules.
16GRAY CAST IRONDuring slow solidification carbon in Fe separates or graphitizes to form separate graphite flakes.
17DUCTILE/NODULAR CAST IRON Mg added to molten iron.Helps to spheroids graphite.Low levels of minor elements such as S and P.
18GENERAL CHARACTERISTICS/ ADVANTAGES OF GRAY CAST IRON Cheap.Low melting point.Fluid – easy to cast, especially advantageous into large complex shapes.Excellent machine ability.Excellent bearing properties.Excellent damping properties.Excellent wear resistance (hi C).Can be heat treated (surface hardened etc.).Can be alloyed etc.Essentially steel + graphite.
19GREAT AT DAMPENINGRelative ability of ferrous metals to dampen vibrations. The energy absorbed per cycle, or specific damping capacity of these can differ by more than 10 times.
20GRAY CAST IRON (EXAMPLE) graphite forms as flakes during solidification.Have γ dendrites + eutectic γ + graphite flakes at T < 1153°C.99% γ + 1 % graphite flakes.
21COMMENTS ON TENSILE PROPERTIES Ferritic – softest; pearlitic – strongest.Variation in elastic modulus.0 ductility – tensile strengths only quoted.C – %, Si %Graphite flake types and size.Fine uniform size wanted, get by:increased superheat to casting.Inoculation with ferrosilicon or calcium silicon.
24DUCTILE/NODULAR CAST IRON Gray iron composition for C and Si.Impurity level control important as it will affect nodule formation.Have nodule instead of flake if we add in 0.05% Mg and/or Ce.As cast structure: graphite forms as nodules instead of flakes.
25NODULAR CAST IRON γ + graphite on cooling below A1 must decide: γ α +Fe3CFavored by slow cooling rates, short diffusion paths etc.γ first follows a) in regions surrounding nodules.Carbon diffuses to existing nodules.As T decreases and diffusion path increases remaining.γ α +Fe3C(pearlite).
26HEAT TREATMENT CONTROL If we want more ductility (less strength) heat.Treat to convert pearlitic areas to α + graphite.Heat to 900°CCool at 20°C/hr from 790° to 650°CFNormal furnace cooling.Could be done as one step with slower.Original cooling.
27CONCLUSIONFinally we concluded that we are all known about the “BASICS OF CAST IRON” which is above in the paper.